Fiber Bragg grating
A fiber Bragg grating (FBG) is a type of
distributed Bragg reflectorconstructed in a short segment of optical fiberthat reflects particular wavelengths of light and transmits all others. This is achieved by adding a periodic variation to the refractive indexof the fiber core, which generates a wavelength specific dielectric mirror. A fiber Bragg grating can therefore be used as an inline optical filterto block certain wavelengths, or as a wavelength-specific reflector.
The first in-fiber Bragg grating was demonstrated by Hill in 1978. [cite journal |last=Hill |first=K.O. |year=1978 |title=Photosensitivity in optical fiber waveguides: application to reflection fiber fabrication |journal=Appl. Phys. Lett. |volume=32 |pages=647 |doi=10.1063/1.89881 ] Initially, the gratings were fabricated using a visible laser propagating along the fiber core. In 1989, Meltz and colleagues demonstrated the modern transverse holographic technique from the side of the fiber utilizing the interference pattern of ultraviolet light. [cite journal |last=Meltz |first=G. |coauthors="et al." |year=1989 |title=Formation of Bragg gratings in optical fibers by a transverse holographic method |journal=Opt. Lett. |volume=14 |pages=823 ]
Fiber Bragg gratings are created by "inscribing" or "writing" the periodic variation of refractive index into the core of an optical fiber using an intense
ultraviolet(UV) source such as a UV laser. Two main processes are used: "interference" and "masking". Which is best depends on the type of grating to be manufactured. A special germanium-doped silica fiber is used in the manufacture of fiber Bragg gratings. The germanium-doped fiber is photosensitive; where the refractive index of the core changes with exposure to UV light, with the amount of change depending on the exposure intensity and duration.
The first manufacturing method, specifically used for uniform gratings, is the use of two-beam
interference. Here the UV laseris split into two beams which interfere with each other creating a periodic intensity distribution along the interference pattern. The refractive index of the photosensitive fiber changes according to the intensity of light that it is exposed to. This method allows for quick and easy changes to the Bragg wavelength, which is a directly related to the interference period, which is a function of the incident angle of the laserlight.
photomaskhaving the intended grating features may also be used in the manufacture of fiber Bragg gratings. The photomask is placed between the UV light source and the photosensitive fiber. The shadow of the photomask then determines the grating structure based on the transmitted intensity of light striking the fiber. Photomasks are specifically used in the manufacture of chirped Fiber Bragg gratings, which cannot be manufactured using an interference pattern.
A single UV
laserbeam may also be used to 'write' the grating into the fiber point-by-point. Here, the laserhas a narrow beam that is equal to the grating period. This method is specifically applicable to the fabrication of long period fiber gratings. Point-by-point is also used in the fabrication of tilted gratings.
Originally, the manufacture of the photosensitive optical fiber and the 'writing' of the fiber Bragg grating were done separately. Today, production lines typically draw the fiber from the
preformand 'write' the grating, all in a single stage. As well as reducing associated costs and time, this also enables the mass production of fiber Bragg gratings. Mass production is in particular facilitating applications in smart structures utilizing large numbers (3000) of embedded fiber Bragg gratings along a single length of fiber.
The grating will typically have a sinusoidal refractive index variation over a defined length. The reflected wavelength (), called the Bragg wavelength, is defined by the relationship,
where is the effective refractive index of the grating in the fiber core and is the grating period. In this case , i.e. it is the average refractive index in the grating (see Fig. 1).
The wavelength spacing between the first minimums (nulls), or the bandwidth (), is given by,
where is the variation in the refractive index (), and is the fraction of power in the core.
The peak reflection () is approximately given by,
where is the number of periodic variations. The full equation for the reflected power (), is given by,
Types of gratings
The term “type” in this context refers to the underlying photosensitivity mechanism by which grating fringes are produced in the fibre. The different methods of creating these fringes have a significant effect on physical attributes of the produced grating, particularly the temperature response and ability to withstand elevated temperatures.Thus far, four types of FBG have been reported with different underlying photosensitivity mechanisms. These are summarised below:
Type I gratings
* Standard grating, written in both hydrogenated and non-hydrogenated fibre of all types
Type I gratings are usually known as standard gratings and are manufactured in fibres of all types under all hydrogenation conditions. Typically, the reflection spectra of a type I grating is equal to 1-T where T is the transmission spectra. This means that the reflection and transmission spectra are complementary and there is negligible loss of light by reflection into the cladding or by absorption. Type I gratings are the most commonly used of all grating types, and the only types of grating available off-the-shelf at the time of writing.
Type IA gratings
* Regenerated grating written after erasure of a type I grating in hydrogenated germanosilicate fibre of all types
Type IA gratings were first published in 2001cite paper | author =Liu, Y. | title =Advanced fibre gratings and their application | publisher =Ph.D. Thesis, Aston University | date =2001 ] during experiments designed to determine the effects of hydrogen loading on the formation of IIA gratings in germanosilicate fibre. In contrast to the anticipated blue shift of the peak Bragg wavelength, a large positive wavelength shift was measured. This type IA grating appeared once the conventional type I FBG had reached saturation followed by subsequent complete or partial erasure, and was therefore labelled as regenerated. It was also noted that the temperature coefficient of the regenerated grating was lower than a standard grating written under similar conditions.
There is a clear relationship between type IA and IIA gratings insomuch as their fabrication conditions are identical in all but one aspect: they both form in B/Ge co-doped fibre but IAs form only in hydrogenated fibres and IIAs form only in non-hydrogenated fibres. [cite paper
author =Simpson, A. G.
title =Optical Fibre Sensors and Their Interrogationdv
publisher =Ph.D. Thesis, Aston University
date =2005] [cite conference
first =A. G.
coauthors =Kalli, K.; Zhou, K.; Zhang, L.; Bennion, I.
title =An ideal method for the fabrication of temperature compensating IA-I strain sensors
pages =postdeadline paper PD4
location =Nara, Japan]
Type II gratings
* Damage written gratings inscribed by high power pulsed lasers. Fringes take the form of physical changes in the crystal lattice
Archambault et al showed that it was possible to inscribe gratings of ~100% (>99.8%) reflectance with a single UV pulse in fibres on the draw tower. The resulting gratings were shown to be stable at temperatures as high as 800˚C. The gratings were inscribed using a single 40mJ pulse from an
excimer laserat 248nm. It was further shown that a sharp threshold was evident at ~30mJ; above this level the index modulation increased by more than two orders of magnitude, whereas below 30mJ the index modulation grew linearly with pulse energy. For ease of identification, and in recognition of the distinct differences in thermal stability, they labelled gratings fabricated below the threshold as type I gratings and above the threshold as type II gratings. Microscopic examination of these gratings showed a periodic damage track at the grating’s site within the fibre  ; hence type II gratings are also known as damage gratings. [cite journal
coauthors =Archambault, J. L.; Reekie, L.; Russell, P. S. J.; Payne, D. N.
title =Single-Pulse Bragg Gratings Written During Fibre Drawing
journal =Electronics Letters
doi =10.1049/el:19931051] [cite journal
first =J. L.
coauthors =Reekie, L.; Russell, P. S. J.
title =100-Percent Reflectivity Bragg Reflectors Produced in Optical Fibres By Single Excimer-Laser Pulses
journal =Electronics Letters
Type IIA gratings
* Regenerated grating written after erasure of a type I grating in hydrogen-free germanosilicate fibres
Later research by Xie et al showed the existence of another type of grating with similar thermal stability properties to the type II grating. This grating exhibited a negative change in the mean index of the fibre and was termed type IIA. The gratings were formed in germanosilicate fibres with pulses from a frequency doubled XeCl pumped dye laser. It was shown that initial exposure formed a standard (type I) grating within the fibre which underwent a small red shift before being erased. Further exposure showed that a grating reformed which underwent a steady blue shift whilst growing in strength. [cite journal
first =W. X.
coauthors =Niay, P.; Bernage, P.; Douay, M.; Bayon, J. F.; Georges, T.; Monerie, M.; Poumellec, B.
title =Experimental-Evidence of 2 Types of Photorefractive Effects Occurring During Photo inscriptions of Bragg Gratings Within Germanosilicate Fibres
journal =Optics Communications
doi =10.1016/0030-4018(93)90127-Q] [cite journal
coauthors =Bernage, P.; Legoubin, S.; Douay, M.; Xie, W. X.; Bayon, J. F.; Georges, T.; Monerie, M.; Poumellec, B.
title =Behaviour of Spectral Transmissions of Bragg Gratings Written in Germania-Doped Fibres - Writing and Erasing Experiments Using Pulsed or CW UV Exposure
journal =Optics Communications
The structure of the FBG can vary via the refractive index, or the grating period. The grating period can be uniform or graded, and either localised or distributed in a superstructure. The refractive index has two primary characteristics, the refractive index profile, and the offset. Typically, the refractive index profile can be uniform or apodized, and the refractive index offset is positive or zero.
There are six common structures for FBGs; [cite journal | last=Erdogan | first=Turan | title=Fiber Grating Spectra | journal=Journal of Lightwave Technology | url=http://ieeexplore.ieee.org/xpl/freeabs_all.jsp?tp=&arnumber=618322&isnumber=13456 | volume=15| issue=8 | pages=1277 – 1294 | month=August | year=1997 | doi=10.1109/50.618322]
# uniform positive-only index change,
# Gaussian apodized,
# raised-cosine apodized,
# discrete phase shift, and
There are basically two quantities that control the properties of the FBG. These are the grating length, , given as,
and the grating strength, . There are, however, three properties that need to be controlled in a FBG. These are the reflectivity, the bandwidth, and the side-lobe strength. From the equation (2) above, we see that the bandwidth depends on the grating strength, and not the grating length. This means the grating strength can be used to set the bandwidth. The grating length, effectively N, can then be used to set the peak reflectivity according to equation (3), which depend on both the grating strength and the grating length. The result of this, is that the side-lobe strength can not be controlled, and this simple optimisation results in significant side-lobes. A third quantity can be varied to help with side-lobe suppression. This is apodization of the refractive index change. The term appodization refers to the grading of the refractive index to approach zero at the end on the grating. Apodized gratings offer significant improvement is side-lobe suppression while maintaining reflectivity and a narrow bandwidth. The two functions typically used to apodize a FBG are Gaussian and raised-cosine.
Chirped fiber Bragg gratings
The refractive index profile of the grating may be modified to add other features, such as a linear variation in the grating period, called a
chirp. The chirp had the effect of broadening the reflected spectrum. The reflected wavelength, given by equation (1), will change relative to any change in the grating period. A grating possessing a chirp has the property of adding dispersion - namely, different wavelengths reflected from the grating will be subject to different delays. This property has been used in the development of phased-arrayantenna systems and polarization mode dispersion compensaiton, as well.
Tilted fiber Bragg gratings
In standard FBGs, the grading or variation of the refractive index is along the length of the fiber (the optical axis), and is typically uniform across the width of the fiber. In a tilted FBG (TFBG), the variation of the refractive index is at an angle to the optical axis. The angle of tilt in a TFBG has an effect on the reflected wavelength, and bandwidth.
Typically the grating period is the same size as the Bragg wavelength, as defined in equation (1). So for a grating that reflects at 1500nm, the grating period is 500nm, using a refractive index of 1.5. Longer periods can be used to achieve much broader responses than are possible with a standard FBG. These gratings are called
long-period fiber grating. They typically have grating periods on the order of 100 micrometers, to a millimeter, and are therefore much easier to manufacture.
The primary application of fiber Bragg gratings is in optical communications systems. They are specifically used as
notch filters. They are also used in optical multiplexersand demultiplexers with an optical circulator, or Optical Add-Drop Multiplexer (OADM). Figure 5 shows 4 channels, depicted as 4 colours, impinging onto a FBG via an optical circulator. The FBG is set to reflect one of the channels, here channel 4. The signal is reflected back to the circulator where it is directed down and dropped out of the system. Since the channel has been dropped, another signal on that channel can be added at the same point in the network.
A demultiplexer can be achieved by cascading multiple drop sections of the OADM, where each drop element uses a FBG set to the wavelength to be demultiplexed. Conversely, a multiplexer can be achieved by cascading multiple add sections of the OADM. FBG demultiplexers and OADMs can also be tunable. In a tunable demultiplexer or OADM, the Bragg wavelength of the FBG can be tuned by strain applied by a
piezoelectric transducer. The sensitivity of a FBG to strain is discussed below in fiber Bragg grating sensors.
Fiber Bragg grating sensors
As well as being sensitive to strain, the Bragg wavelength is also sensitive to
temperature. This means that fiber Bragg gratings can be used as sensing elements in optical fiber sensors. In a FBG sensor, the measurand causes a shift in the Bragg wavelength, . The relative shift in the Bragg wavelength, , due to an applied strain () and a change in temperature () is approximately given by,
Here, is the "coefficient of strain", which is related to the "strain optic coefficient" . Also, is the "coefficient of temperature", which is made up of the "thermal expansion coefficient" of the optical fiber, , and the "thermo-optic coefficient", [cite book |last=Andreas |first=O. |coauthors=Kyriacos, K. |year=1999 |title=Fiber Bragg Grating. Fundamentals and Applications in Telecommunications and Sensing |publisher=Artech House ] .
Fiber Bragg gratings can then be used as direct sensing elements for strain and temperature. They can also be used as transduction elements, converting the output of another sensor, which generates a strain or temperature change from the measurand, for example fiber Bragg grating gas sensors use an absorbent coating, which in the presence of a gas expands generating a strain, which is measurable by the grating. Technically, the absorbent material is the sensing element, converting the amount of gas to a strain. The Bragg grating then transduces the strain to the change in wavelength.
Specifically, fiber Bragg gratings are finding uses in instrumentation applications such as
seismologyand as downhole sensors in oil and gas wells for measurement of the effects of external pressure, temperature, seismic vibrations and inline flow measurement. As such they offer a significant advantage over traditional electronic gauges used for these applications in that they are less sensitive to vibration or heat and consequently are far more reliable.
Long-period fiber grating
Photonic crystal fiber
Distributed temperature sensingby fiber optics
* [http://bit.or.at/irca/bbsshow8.php?ref1=OO/INTA/36&vQuelle=&bcc= Bragg grating as hydrogen detector]
Wikimedia Foundation. 2010.
Look at other dictionaries:
Bragg diffraction — (also referred to as the Bragg formulation of X ray diffraction) was first proposed by William Lawrence Bragg and William Henry Bragg in 1913 in response to their discovery that crystalline solids produced surprising patterns of reflected X rays… … Wikipedia
Fiber optic sensor — A fiber optic sensor is a sensor that uses optical fiber either as the sensing element ( intrinsic sensors ), or as a means of relaying signals from a remote sensor to the electronics that process the signals ( extrinsic sensors ). Fibers have… … Wikipedia
Bragg's law — In physics, Bragg s law is the result of experiments into the diffraction of X rays or neutrons off crystal surfaces at certain angles, derived by physicist Sir William Lawrence Bragg [ There are some sources, like the Academic American… … Wikipedia
Bragg-Gitter — Lichtwellenleiter mit Bragg Gitter Λ = Gitterperiode, n = Brechzahl, PI = Eingangsleistung, PB = reflektierte Leistung, PT = durchgehende Leistung, λ = Wellenlänge des Lichts Faser Bragg Gitter sind in Lichtwellenleiter eingeschriebene optische… … Deutsch Wikipedia
Bragg-Reflektor — Lichtwellenleiter mit Bragg Gitter Λ = Gitterperiode, n = Brechzahl, PI = Eingangsleistung, PB = reflektierte Leistung, PT = durchgehende Leistung, λ = Wellenlänge des Lichts Faser Bragg Gitter sind in Lichtwellenleiter eingeschriebene optische… … Deutsch Wikipedia
Fiber laser — A fiber laser or fibre laser is a laser in which the active gain medium is an optical fiber doped with rare earth elements such as erbium, ytterbium, neodymium, dysprosium, praseodymium, and thulium. They are related to doped fiber amplifiers,… … Wikipedia
Photonic-crystal fiber — (PCF) is a new class of optical fiber based on the properties of photonic crystals. Because of its ability to confine light in hollow cores or with confinement characteristics not possible in conventional optical fiber, PCF is now finding… … Wikipedia
Distributed Bragg reflector — A distributed Bragg reflector (DBR) is a reflector used in waveguides, such as optical fibers. It is a structure formed from multiple layers of alternating materials with varying refractive index, or by periodic variation of some characteristic… … Wikipedia
Long-period fiber grating — A long period fiber grating is an optical fiber structure with the properties periodically varying along the fiber, such that the conditions for the interaction of several copropagating modes are satisfied. The period of such a structure is of… … Wikipedia
Optical fiber — A bundle of optical fibers A TOSLINK fiber optic audio c … Wikipedia